journal of crystal growth - atwater research group 2014-12-23آ a1. crystal structure a1. high...
Post on 04-Jul-2020
Embed Size (px)
Single phase, single orientation Cu2O (1 0 0) and (1 1 0) thin films grown by plasma-assisted molecular beam epitaxy
Yulia Tolstova n, Samantha S. Wilson, Harry A. Atwater Thomas J. Watson Laboratories of Applied Physics, California Institute of Technology, Pasadena, CA 91125, United States
a r t i c l e i n f o
Article history: Received 16 July 2014 Received in revised form 15 October 2014 Accepted 21 October 2014 Communicated by R. Fornari Available online 30 October 2014
Keywords: A1. Crystal structure A1. High resolution X-ray diffraction A3. Molecular beam epitaxy B1. Oxides B2. Semiconducting materials
a b s t r a c t
Epitaxial growth of cuprous oxide (Cu2O) has been achieved on (1 0 0) and (1 1 0) orientations of MgO by plasma-assisted molecular beam epitaxy. Growth was investigated using a pure oxygen plasma as well as a 90%Ar/10%O2 plasma. Cu2O films grown using pure oxygen on MgO (1 0 0) have a limited growth window and typically exhibit multiple phases and orientations. Films grown on MgO (1 1 0) using pure oxygen are phase stable and predominantly (1 1 0) oriented, with some (2 0 0) orientation present. Films grown using an Ar/O2 plasma on MgO (1 0 0) have improved phase stability and a single (1 1 0) orientation. Growth on MgO (1 1 0) using an Ar/O2 plasma yields highly reproducible (1 1 0) oriented single phase Cu2O films with a much wider growth window, suggesting that this substrate orientation is preferable for Cu2O phase stability.
& 2014 Elsevier B.V. All rights reserved.
Cuprous oxide (Cu2O) was one of the first semiconductors to be studied, and many of its bulk properties have since been elucidated. In the past few decades, Cu2O gained attention as an earth-abundant semiconductor with promising photovoltaic properties including high absorption and long minority carrier diffusion length around 5 μm [1,2]. It is composed of non-toxic elements and can be easily fabricated by thermal oxidation of Cu foils. While the bulk properties of Cu2O are attractive for photovoltaic applications, surface stability has been one of the most pressing issues to achieve a high efficiency solar cell. Cu2O is intrinsically p-type and thus requires a hetero- junction partner to form a solar cell with a high open circuit voltage, which introduces the possibility of heterojunction interface defects. Cu2O devices are highly susceptible to deleterious interface reactions which impede high cell performance [3,4]. The highest reported photovoltaic efficiency for a Cu2O absorber device is 5.38% , while the detailed balance limit has been calculated to exceed 20% . One of the main reasons for low efficiency is phase instability of the Cu2O surface, coupled with a small heat of formation (�170 kJ/mol) and a low electron affinity (3.2 eV). A thermodynamic phase diagram for the Cu–O system can be found in .
Arguably the strongest motivation for Cu2O in photovoltaic applications is its relatively large band gap of 2.1 eV (and exciton
gap at 1.9 eV), which make it a promising candidate as a top cell in a tandem solar cell combined with a crystalline silicon bottom cell. In order for such a tandem cell to improve upon existing Si cell efficiency, a Cu2O cell efficiency approaching 10% is required . The development of such a structure would require synthesis by thin film methods, and molecular beam epitaxy (MBE) provides precise control over many deposition parameters and generally yields high quality material. MBE synthesis of Cu2O on MgO substrates has been demonstrated using pure atomic oxygen [7–9], however no reports of a diluted oxygen plasma have been made to date. Also, growth on MgO (1 1 0) surface has been reported by sputtering  and pulsed laser deposition , but not by MBE. DFT calculations  show that the Cu2O (1 1 0) surface has the lowest energy, so it is reasonable to assume that a substrate that promotes growth in this direction may foster Cu2O phase stability over a larger range of deposition parameters, and this is consistent with results of this work. We compare the structural properties of Cu2O films grown using a pure oxygen atmosphere to films grown using a 90%Ar/10%O2 premix, on (1 0 0) and (1 1 0) orientations of MgO.
2. Experimental details
Thin films of CuxO were grown in a custom molecular beam epitaxy system equipped with an Oxford RF atom source. RF atom sources dissociate molecular species (such as O2 or N2) into atomic species for increased reactivity while minimizing ionic species
Contents lists available at ScienceDirect
journal homepage: www.elsevier.com/locate/jcrysgro
Journal of Crystal Growth
http://dx.doi.org/10.1016/j.jcrysgro.2014.10.045 0022-0248/& 2014 Elsevier B.V. All rights reserved.
n Corresponding author. E-mail address: firstname.lastname@example.org (Y. Tolstova).
Journal of Crystal Growth 410 (2015) 77–81
www.sciencedirect.com/science/journal/00220248 www.elsevier.com/locate/jcrysgro http://dx.doi.org/10.1016/j.jcrysgro.2014.10.045 http://dx.doi.org/10.1016/j.jcrysgro.2014.10.045 http://dx.doi.org/10.1016/j.jcrysgro.2014.10.045 http://crossmark.crossref.org/dialog/?doi=10.1016/j.jcrysgro.2014.10.045&domain=pdf http://crossmark.crossref.org/dialog/?doi=10.1016/j.jcrysgro.2014.10.045&domain=pdf http://crossmark.crossref.org/dialog/?doi=10.1016/j.jcrysgro.2014.10.045&domain=pdf mailto:email@example.com http://dx.doi.org/10.1016/j.jcrysgro.2014.10.045
which typically have high kinetic energies and are associated with creation of point defects. Ionic components of the plasma that escape the atom source were further filtered out by ion deflection plates. Thus the current of gas species was composed of atomic argon and/or oxygen. Oxygen (Air Liquide, 99.9999% purity) partial pressure was varied between 1�10�7 and 1�10�5 Torr. For growths with argon/oxygen premix (Air Liquide, 99.9999% purity, 10.0% oxygen, balance argon), the gas partial pressure of argon was correspondingly an order of magnitude higher. The presence of argon allowed for stability of the plasma, while decreasing the partial pressure of reactive oxygen species. Partial pressures were monitored by a residual gas analyzer (RGA). Atom source plasma power was varied between 100 and 200 W and plasma optical emission voltage ranged from 1 V to 3 V during film deposition. Plasma emission voltage corresponds to the intensity of light emitted from the plasma and correlates with the efficiency of dissociation of the molecular gas into its atomic components. The growth chamber base pressure was o3� 10�9 Torr. Copper metal (6 N, Alfa Aesar) was evaporated from a high temperature effusion cell at a temperature ranging from 1250 to 1300 1C. CuxO was formed reactively at the surface of the substrate kept at a temperature ranging from 400 to 650 1C. MgO was chosen as a substrate because it is the closest lattice matched commercially available single crystal; it is also refractory, transparent, and non- conductive, which makes it suitable for a variety of electrical and
optical characterization techniques. MgO substrates were cleaned in situ by annealing at deposition temperature for an hour and subsequently plasma cleaned for 10 minutes. In situ reflection high energy electron diffraction (RHEED, with electron beam energy of 15 keV) was used to confirm cleanliness and orientation of the substrate surface and monitor film structure at various stages of the growth. Ex situ characterization included high resolution X-ray diffraction (HRXRD, Panalytical XPert Pro), transmission electron microscopy (TEM, FEI Tecnai F30 with S-TWIN objective, 300 keV electron energy), and atomic force microscopy (AFM, Asylum Research MFP 3D). TEM cross sections were prepared using standard focused ion beam milling on an FEI Versa 3D.
3. Results and discussion
3.1. Growth using pure oxygen plasma
Growth of CuxO on MgO was initially studied by varying oxygen partial pressure (using pure oxygen gas) and substrate tempera- ture, while fixing the Cu effusion cell temperature at 1275 1C, atom source plasma power at 100 W, and plasma optical emission voltage at 1 V (which corresponds to the lower range of stability of the plasma source). As illustrated in Fig. 1(a, b), the growth window for the Cu2O phase on MgO (1 0 0) was found to be too
Fig. 1. HRXRD spectra of CuxO films grown on MgO (1 0 0) at (a) 1�10�6 Torr and (b) 5�10�6 Torr oxygen, both cases corresponding to the presence of undesirable phases and (c) pure phase Cu2O film grown on MgO (1 1 0) at 9�10�6 Torr.
Fig. 2. RHEED images of Cu2O growth on MgO using pure oxygen plasma. (a) Plasma cleaned MgO (1 0 0) surface along the [1 1 0] azimuth; (b) 100 nm of Cu2O showing growth initiates and persists in the Volmer–Weber or island regime and the pattern is a superposition of the Cu2O ½1 1 1� and ½2 1 1� zone axis transmission patterns; (c) indexing of diffraction spots in (b) along ½1 1 1� zone axis (black) and ½2 1 1� zone axis (gray); (d) plasma cleaned MgO (1 1 0) surface along the [1 1 1] azimuth; (e) 10 nm of Cu2O along ½1 1 1� again initiates with island growth (for spot indexing refer to Fig. 5f); (f) after 100 nm of Cu2O viewed along ½1 1 1�, islands merge into a smooth film with steps, as evidenced by a streaky pattern.
Y. Tolstova et al. / Journal of Crystal Growth 410 (2015) 77–8178
narrow to reproducibly grow single phase films. Raising the pressure of oxygen by only half an order of magnitude, while maintaining otherwise identical growth parameters and low oxy- gen plasma power, changed the film composition from a mixture of Cu2O and Cu to CuO. Fig. 1(c) shows that single-phase epitaxial growth of Cu2O on MgO (1 1 0) is ach